drain, transistor channel, and polysilicon
Flash Memory Scaling Al Fazio
control gate terminals. Any charge present
on the floating gate is retained due to the
inherent Si-SiO2 energy barrier height,
leading to the nonvolatile nature of the
memory cell. Characteristic of the struc-
ture is a thin tunneling oxide ( 100 Å), an
oxide/nitride/oxide (ONO) interpoly di-
electric (IPD) that resides between the two
polysilicon gates, and a short electrical
Abstract channel length. Because the only electrical
In order to meet technology scaling in the field of solid-state memory and data connection to the floating gate is through
storage, the mainstream transistor-based flash technologies will start evolving to capacitors, the flash cell can be thought
incorporate material and structural innovations. Dielectric scaling in nonvolatile of as a linear capacitor network with an
memories is approaching the point where new approaches will be required to meet the n-channel transistor attached. The thresh-
scaling requirements while simultaneously meeting the reliability and performance old voltage of the device can be changed
requirements of future products. High-dielectric-constant materials are being explored as by modifying the charge on the floating
possible candidates to replace the traditional SiO2 and ONO (oxide/nitride/oxide) films gate, which can retain this charge for many
used today in memory cells. Likewise, planar-based memory cell scaling is approaching years. Data can be stored in the memory
the point where scaling constraints force exploration of new materials and nonplanar,
by adding or removing charge. In the sim-
plest form of a memory cell, two threshold
three-dimensional scaling alternatives. This article will review the current status and
levels (high and low) can store one bit of
discuss the approaches being explored to provide scaling solutions for future transistor
information in each cell. This concept can
floating-gate-based nonvolatile memory products. Based on the introduction of material
be extended to store more levels, com-
innovations, it is expected that the planar transistor-based flash memory cells can scale monly called an MLC (multilevel cell).3
through at least the end of the decade (2010) using techniques that are available today Four levels would allow two bits of data
or projected to be available in the near future. More complex, structural innovations will per cell to be stored. Adding and remov-
be required to achieve further scaling. ing charge from the floating gate is nor-
mally achieved by Fowler–Nordheim
Keywords: flash memory, floating gates, nonvolatile memory, scaling. tunneling or hot carrier injection.
Flash Cell Programming
Programming a flash cell means that
Introduction charge, or electrons, are added to the float-
Floating gate flash memory1,2 is now the major scaling challenges for flash memory ing gate. Figure 2 shows the cell bias con-
fastest-growing memory segment, driven and identify some of the potential solu- ditions during program operation. A high
by the rapid growth of portable devices tions to enable further scaling to occur. drain-to-source bias voltage is applied,
such as digital cameras and cellular phones. along with a high control gate voltage. The
The technology allows for data stored in Flash Cell Basic Operation gate voltage inverts the channel (turns it to
multiple memory cells to be erased in a A floating gate nonvolatile flash memory the ON state), while the drain bias acceler-
single action (a “flash”) by means of an cell is shown schematically in Figure 1. It ates electrons toward the drain. Program-
applied voltage. Flash memory is catego- is a metal oxide semiconductor (MOS) tran- ming a flash cell by channeling electrons
rized into two basic approaches: NOR flash, sistor with two gates, a floating gate and a with high kinetic energy—so-called hot
characterized by a fast initial access time control gate. The memory cell consists of electrons—can be understood by use of the
for high read performance; and NAND an n-channel transistor with the addition “lucky” electron model,4 as illustrated by
flash, characterized by a slow initial access of an electrically isolated polysilicon float- the energy-band diagram in Figure 3. In
time and high write performance. This ar- ing gate. Electrical access to the floating the model, an electron crosses the channel
ticle will focus on the scaling of NOR flash gate is only through a capacitor network without collision—a process that requires
memory; however, many of the scaling con- of surrounding SiO2 layers and source, some luck—thereby gaining sufficient
siderations described in this article are com- kinetic energy to surmount the 3.2 eV
mon to both NOR and NAND floating-gate Si-SiO2 energy barrier. Prior to entering the
flash memories. drain and being swept away, this lucky
As flash memory devices begin to scale electron experiences a collision with the
into the sub-100-nm lithography regime,
scaling is becoming a greater challenge due
to the high electric fields required for the
programming and erase operations and the
stringent leakage requirements for long-
term charge storage. These requirements
are imposing fundamental scaling limita-
tions on the cell operating voltages and on
the physical thickness of the tunneling di-
electric. Overcoming these limitations will
require innovations in cell structure and Figure 1. Flash memory cell: cross Figure 2. Memory cell bias conditions
device materials. This article will outline the section along the channel. for programming.
814 MRS BULLETIN/NOVEMBER 2004
Flash Memory Scaling
Flash Memory Scaling Challenges
Figure 6 depicts the layout of a flash mem-
ory cell and some of the major scaling
constraints. Throughout the history of the
development of flash, the cell size has been
reduced through a combination of litho-
graphy and self-alignment techniques.6
Today, it is common for many of the cell
components to be fully or partially self-
aligned, eliminating the need for lithography
registration between layers. Figure 7 illus-
trates various self-alignment techniques
that have been deployed. Once the cell be-
Figure 3. Energy-band diagram for comes fully self-aligned, further scaling is
channel hot-electron programming. Ec is largely determined by the electrical limiters
the energy of the conducting band and of the cell, where scaling the flash cell re- Figure 5. Energy-band diagram for
Ev is the energy of the valence band. Fowler–Nordheim tunneling erase
quires scaling the cell’s capacitive network operation.
and basic transistor features. The following
sections explore how the introduction of
silicon lattice and is redirected toward the new materials and structures will enable
Si-SiO2 interface with the aid of the gate flash memory to continue scaling beyond gramming. Figure 9 shows an example of a
field. The electron is subsequently captured simple linear extrapolations. “finfet” (a MOS field-effect transistor made
on the floating gate and retained as stored in a fin structure) type of flash cell with a
charge. Channel-Length Scaling: vertical storage gate. This structure moves
Challenges and Alternatives the channel-length constraint into the verti-
Erasing a Flash Cell To achieve hot carrier programming, a cal (z) direction, allowing further x–y scaling
As mentioned earlier, in a flash cell, the voltage of about 4 V is required from the to occur.
contents of the memory, or charge, are re- drain to source to produce electrons of high
moved by means of applying an electrical enough energy to overcome the 3.2 eV Capacitor Network Scaling
voltage, erasing them in a “flash.” The Si-SiO2 barrier height. One can extrapolate Challenges and Alternatives
electrical erasure of flash memory is the historical scaling trend for channel Maintaining adequate coupling of the
achieved by Fowler–Nordheim tunneling,5 length and extrapolate potential limits. This control gate to the floating gate is a key as-
for which the bias conditions are shown in extrapolation is based on the fact that the pect in scaling the cell channel. This is re-
Figure 4. Under these conditions, a high basic planar cell structure is the same for all quired to keep the erase voltage as low as
field (8–10 MV/cm) is present between of the generations, and scaling is achieved possible, avoid erase saturation, and pro-
the floating gate and the channel. As evi- by reducing specific cell dimensions. The vide control of the channel for reading and
denced by the energy-band diagram of difference between the gate length Lgate and programming. Erase saturation occurs
Figure 5, electrons tunneling through the the effective electrical gate length Leff is the when the field across the interpoly dielec-
first 30 Å of the SiO2 are then swept into lateral diffusion of the source and drain tric is equal to the field in the tunnel oxide,
the silicon. When the erase operation has underneath the gate. The convergence point so that for each electron that is removed
been completed, electrons have been re- of the trend represents a projection of a (erased) from the floating gate, another
moved from the floating gate, reducing scaling rate limiter of the current planar electron is added through the IPD. As the
the cell threshold. While programming is cell structure. As shown in Figure 8, scaling cell scales and self-aligned techniques are
selective to each individual cell, erasing is the gate length will be limited below the used for the floating gate, maintaining con-
not, with many cells (typically, 64 kbytes) 70 nm lithography node due to the inabil- trol of the channel requires a thinner IPD
being erased simultaneously. ity of the shorter channel length to with- between the control gate and the floating
stand the required programming voltage. gate, approaching the thickness of the tun-
To continue scaling at the same rate, more neling dielectric. The requirement of an IPD
revolutionary ideas will be needed to scale is to provide good capacitive coupling to
the Leff more aggressively. the floating gate from the control gate, while
Scaling the channel length could be minimizing any leakage through the di-
achieved through engineering of the Si-SiO2 electric. Unlike the tunnel oxide, this di-
barrier. By choosing dielectric alternatives electric stack is not expected to support
to SiO2, the barrier can be tailored to allow charge transfer during programming and
hot-electron injection to occur at lower erase operations. For the last decade, the
voltages. Some promising alternatives have IPD has been composed of an ONO sand-
been proposed.7 Three-dimensional struc- wich film. ONO scaling has been achieved
tures8 are an alternative way to address the by thinning the dielectrics while maintain-
gate-length scaling constraint. Both “fin” ing control of the thickness. This scaling has
Figure 4. Memory cell bias conditions
(protruding above the silicon like a fish’s also been enabled by improving the quality,
for erase operation. The floating gate is fin) and “U” (a U-shaped trough etched in terms of the number of imperfections, of
the rectangle in the middle, and the below the silicon surface) structures show the oxide on the floating gate, which can be
channel is the region between the n promise to allow further scaling while main- aided by reducing the floating-gate poly-
areas at the top of the substrate layer. taining the channel length required for pro- silicon surface roughness.
MRS BULLETIN/NOVEMBER 2004 815
Flash Memory Scaling
An alternative approach would be to tions include Al2O3 with a TaN gate that
replace the IPD with a higher-dielectric- has been proposed for a SONOS-type
constant material as compared to SiO2. To memory device,9 that could in principle be
maintain the high capacitive coupling im- deployed in a floating-gate device as well.
provement, a metal gate would be required However, the gate electrode should be
to reduce the series capacitance from gate chosen consistent with the high- film to
depletion. Since this film is not expected to make sure the energy barrier is engi-
transport charge (as is the case with the neered to reduce carrier injection.
tunnel oxide), it has fewer constraints and Another scaling limitation of a capacitor
it may be easier to find a candidate to meet network is the communication of two
the cell requirements, as compared with adjacent cells through the capacitance be-
replacing the tunnel oxide. Possible op- tween the cells. As the spacing between Figure 8. Gate-length scaling projection.
Lgate is the gate length; Leff is the effective
electrical gate length.
floating gates is reduced, coupling between
floating gates increases; thus, the data
stored in one cell can influence the opera-
tion of an adjacent cell (Figure 10). Com-
munication between adjacent cells may be
reduced through a reduction in the thick-
ness of the floating gate and control gate,
thus reducing the area of the capacitor.
Alternative nonconducting floating gate
structures are being actively investigated
in the industry as ways to replace the nor-
mally conducting floating gate with non-
conducting floating nodes. The two main
thrusts in this area are silicon nitride stor-
age10 and nanocrystal storage, including
metal-based and semiconductor nano-
crystals.11 While these approaches offer the
Figure 6. Flash cell layout and major scaling constraints. The lighter-green areas are flash possibility of replacing the floating gate,
cell gates. both require significant changes in proc-
essing, cell operation (program, erase, read)
and structure in order to achieve a viable
memory. As such, these approaches face
significant barriers to becoming mainstream
alternatives to floating gate storage.
Tunnel Oxide Scaling Challenges
Scaling of the tunneling oxide is a pri-
mary limitation to cell scaling. The tunnel
Figure 7. Self-alignment techniques. Use of a self-aligned source (SAS), self-aligned poly (SAP) Figure 9. Three-dimensional
floating gate, and unlanded contact (ULC) eliminates most lithography registration components “finfet”(fin-shaped field-effect transistor)
of the flash cell area.The dotted box represents one unit memory cell within an array. is the flash structure with a vertical storage
minimum lithography feature size; ILD interlayer dielectric; STI shallow trench isolation. transistor.
816 MRS BULLETIN/NOVEMBER 2004
Flash Memory Scaling
1. W. Brown and J. Brewer, Nonvolatile Semicon-
ductor Memory Technology: A Comprehensive
Guide to Understanding and Using NVSM Devices
(IEEE Press, New York, 1998).
2. V.N. Kynett, A. Baker, M.L. Fandrick, G.P.
Hoekstra, O. Jungroth, J.A. Kreifels, S. Wells,
and M.D. Winston, “An In-System Reprogram-
mable 256 K CMOS Flash Memory,” Tech. Dig.
IEEE Int. Solid-State Circuits Conf. (1988) p. 132.
3. M. Bauer, R. Alexis, G. Atwood, B. Baltar,
A. Fazio, K. Frary, M. Hensel, M. Ishac, J.
Javanifard, M. Landgraf, D. Leak, K. Loe, D. Mills,
P. Ruby, R. Rozman, S. Sweha, S. Talreja, and K.
Wojciechowski, “A Multilevel-Cell 32 Mb Flash
Memory,” Tech. Dig. IEEE Int. Solid-State Circuits
Figure 10. Capacitive coupling between Conf. (1995) p. 132.
neighboring cells. 4. S. Tam, P.K. Ko, and C. Hu, “Lucky Electron
Model of Channel Hot Electron Injection in
MOSFETs,” IEEE Trans. Electron. Dev. (Septem-
oxide needs to scale to enable channel- ber 1984).
length scaling, but this is not possible, due 5. M. Lenzlinger and E.H. Snow, J. Appl. Phys.
to data retention requirements. The charge 40 (1) (January 1967) p. 278.
6. A. Fazio, S. Keeney, and S. Lai, Intel Technol.
retention requirements set a lower limit for
J. (May 2002), accessible at developer.intel.com/
tunnel oxide thickness of about 80 Å, due technology/itj/2002/volume06issue02/ (accessed
to stress-induced low-field tunneling,12 as October 2004).
shown in Figure 11. In fact, the Interna- 7. M. She, T.-J. King, C. Hu, W. Zhu, Z. Luo, J.-P.
tional Technology Roadmap for Semicon- Han, and T.-P. Ma, Proc. 2001 Int. Semicond. Dev.
ductors (ITRS) revealed a tunnel oxide Res. Symp. (2001) p. 641.
scaling roadmap that was made more con- 8. H.B. Pein and J.D. Plummer, Tech. Dig. 1993
servative in the 2001 edition due to the IEEE Int. Electron. Dev. Meet. (1993) p. 11.
challenges in going below 80 Å. It is be- 9. C.-H. Lee, K.-I. Choi, M.-K. Cho, Y.-H. Song,
K.-C. Park, and K. Kim, “A Novel SONOS
coming clear that to enable a significant
Structure of SiO2SiNAl2O3 with TaN Metal Gate
reduction below 80 Å, a significant change Figure 12. (a) Classical single barrier
for Multi-Gigabit Flash Memories,” Tech. Dig.
in the SiO2 dielectric is required. Alternative shows that tunneling is modulated by
2003 IEEE Int. Electron. Dev. Meet. (2003).
materials are being explored to allow fur- the barrier width. With barrier engineering,
10. B. Eitan, P. Pavan, I. Bloom, E. Aloni, A.
ther scaling of the tunneling dielectric. In it is possible to have (b) a lower barrier
Frommer, and D. Finzi, Electron. Dev. Lett. 21
under high field and (c) a higher barrier
particular, “crested barrier”13,14 composite under low field.14 U energy barrier
(11) (2000) p. 543.
films may have promise in enabling the de- 11. J. De Blauwe, “Nanocrystal Nonvolatile
height; d distance.
sign of a more optimal barrier structure. Memory Devices,” IEEE Trans. Nanotechnol. 1
With SiO2, or any material with a uniform (1) (March 2002) p. 72.
12. K. Naruke, S. Taguchi, and M. Wada, IEDM
barrier, the high transparency at electric barrier height reduces under the high-field
Tech. Dig. (1988) p. 424.
fields necessary for fast program and erase condition when charge transport is de- 13. A. Korotkov and K. Likharev, IEDM Tech.
operations ( 10 MV/cm) cannot be sired, but increases again when a low field Dig. (1999) p. 223.
achieved along with low transparency at is present, reducing the low-field leakage 14. K.K. Likharev, IEEE Circuits Dev. Mag. 16
fields (1–3 MV/cm) where good retention current and improving retention. (4) (July 2000) p. 16. ■
is required. The reason for this is that the
barrier height remains fixed regardless of Summary
the applied electric field, and field emission Flash memory devices are now pushing
occurs due to thinning of the barrier width into the sub-100-nm lithography regime.
(Figure 12a). If a triangular or crested barrier Device scaling is becoming challenging due MRS Future Meetings
approach is used (Figure 12b), then the to the high electric fields required for the
programming and erase operations and the
stringent leakage requirements for long- for the latest Information on
term charge storage. Overcoming these MRS Meetings and sponsored
limitations will require innovations in cell
structure and device materials. Three- workshops, check out our
dimensional structures and self-alignment Web site at:
techniques can address the physical scaling
issues. High-dielectric-constant and crested www.mrs.org/meetings/
barrier (or barrier-engineered) materials
can address the dielectric scaling issues. It
is projected that flash scaling can progress
at the current rate through at least the end
of the decade (2010) using techniques that See page 893!
Figure 11. Stress-induced leakage are available today or projected to be
current in thin oxides.12 available in the near future.
MRS BULLETIN/NOVEMBER 2004 www.mrs.org/publications/bulletin 817